Presentation on theme: "8 Forms of Corrosion: Uniform Pitting"— Presentation transcript:
18 Forms of Corrosion: Uniform Pitting Crevice Corrosion or Concentration CellGalvanic or Two-MetalStress Corrosion CrackingIntergranularDealloyingErosion Corrosion
2Galvanic Corrosion:Possibility when two dissimilar metals are electrically connected in an electrolyte*Results from a difference in oxidation potentials of metallic ions between two or more metals. The greater the difference in oxidation potential, the greater the galvanic corrosion.Refer to Galvanic Series (Figure 13-1)The less noble metal will corrode (i.e. will act as the anode) and the more noble metal will not corrode (acts as cathode).Perhaps the best known of all corrosion types is galvanic corrosion, which occurs at the contact point of two metals or alloys with different electrode potentials.*Meet requirements of a corrosion cell!! See slide 4
3Galvanic Series:Questions:Worst combination?Aluminum and steel?Titanium and Zinc?Stainless Steel and Copper?Mild steel and cast iron?Show Demo!
4Note, positions of ss and al** GALVANIC SERIESGalvanic Series in Seawater (supplements Faraq Table 3.1 , page 65), EIT Review Manual, page 38-2Tendency to be protected from corrosion, cathodic, more noble endMercuryPlatinumGoldZirconium GraphiteTitaniumHastelloy C MonelStainless Steel (316-passive)Stainless Steel (304-passive)Stainless Steel (400-passive)Nickel (passive oxide)SilverHastelloy 62Ni, 17CrSilver solderInconel 61Ni, 17CrAluminum (passive AI203)70/30 copper-nickel90/10 copper-nickelBronze (copper/tin)CopperBrass (copper/zinc)Alum Bronze Admiralty BrassNickelNaval Brass TinLead-tinLeadHastelloy AStainless Steel (active)Lead Tin SolderCast ironLow-carbon steel (mild steel)Manganese UraniumAluminum AlloysCadmiumAluminum ZincBerylliumMagnesiumPASSIVE – will not corrode – act as cathode. These elements are least likely to give up electrons!Note, positions of ss and al**ACTIVE – will corrode – act as anode. These elements most likely to give up electrons!
6Galvanic Corrosion Potentials: Figure 1. A bi-metal corrosion cell. The corrosion potential is the potential to which the metal falls relative to a hydrogen standard.Figure 2. Standard reduction potentials of metals.Galvanic Corrosion Potentials:Figure 1 illustrates the idea of an electro-chemical reaction. If a metal is placed in a conducting solution like salt water, it dissociates into ions, releasing electrons, as the iron is shown doing in the figure, via the ionization reactionFe Fe e-The electrons accumulate on the iron giving it a negative charge that grows until the electrostatic attraction starts to pull the Fe++ ions back onto the metal surface, stifling further dissociation. At this point the iron has a potential (relative to a standard, the hydrogen standard) of –0.44 volts. Each metal has its own characteristic corrosion potential (called the standard reduction potential), as plotted in Figure 2.If two metals are connected together in a cell, like the iron and copper samples in Figure 1, a potential difference equal to their separation on Figure 2 appears between them. The corrosion potential of iron, -0.44, differs from that of copper, , by 0.78 volts, so if no current flows in the connection the voltmeter will register this
7Liquid Cell Battery:dry cell is a galvanic electrochemical cell with a pasty low-moisture electrolyte. A wet cell, on the other hand, is a cell with a liquid electrolyte, such as the lead-acid batteries in most cars
8Dry Cell - Zinc-carbon battery Zn(s) → Zn2+(aq) + 2 e- - oxidation reaction that happens at zinc = anode2MnO2(s) + 2 H+(aq) + 2 e- → Mn2O3(s) + H2O(l)- reduction reaction at carbon rod = cathode
9Design for Galvanic Corrosion? Material Selection: Do not connect dissimilar metals! Or if you can’t avoid it:Try to electrically isolate one from the other (rubber gasket).Make the anode large and the cathode smallBad situation: Steel siding with aluminum fastenersBetter: Aluminum siding with steel fastenersEliminate electrolyteGalvanic of anodic protection
10Design for Galvanic Corrosion? Galvanic severity depends on:NOTNot amount of contactNot volumeNot massAmount of separation in the galvanic seriesRelative surface areas of the two. Severe corrosion if anode area (area eaten away) is smaller than the cathode area. Example: dry cell battery
11Steel bolt (less noble) is isolated from copper plates. See handout! – Read Payer video HO
12Stress Corrosion Cracking: Spontaneous corrosion induced cracking of a material under static (or residual) tensile stress.Problem w/ parts that have residual stress – stamping double whammy – residual stress at bends = SCC + stress concentration.AKA environmentally assisted cracking (EAC), other forms:Hydrogen embrittlementCaustic embrittlementLiquid metal corrosion
13Factors: Must consider metal and environment. What to watch for: Stainless steels at elevated temperature in chloride solutions.Steels in caustic solutionsAluminum in chloride solutions3 Requirements for SCC:Susceptible alloyCorrosive environmentHigh tensile stress or residual stress
14Design for Stress Corrosion Cracking: Material selection for a given environment (Table 13-2).Reduce applied or residual stress - Stress relieve to eliminate residual stress (i.e. stress relieve after heat treat).Introduce residual compressive stress in the service.Use corrosion alloy inhibitors.Apply protective coatings.
15Stress Corrosion Cracking: See handout, review HO hydron!
16Intergranular Attack: Corrosion which occurs preferentially at grain boundries.Why at grain boundries?Higher energy areas which may be more anodic than the grains.The alloy chemistry might make the grain boundries dissimilar to the grains. The grain can act as the cathode and material surrounding it the anode.
17Intergranular Attack: How to recognize it?Near surfaceCorrosion only at grain boundries (note if only a few gb are attacked probably pitting)Corrosion normally at uniform depth for all grains.
18Example 1: Intergranular Attack: Sensitization of stainless steels:Heating up of austenitic stainless steel (750 to 1600 F) causes chromuim carbide to form in the grains. Chromuim is therefore depleted near the grain boundries causing the material in this area to essentially act like a low-alloy steel which is anodic to the chromium rich grains.
19Example: Intergranular Attack: Sensitization of stainless steels:Heating up of austenitic stainless steel (750 to 1600 F) causes chromuim carbide to form in the grains. Chromuim is therefore depleted near the grain boundries causing the material in this area to essentially act like a low-alloy steel which is anodic to the chromium rich grains.Preferential Intergranular Corrosion will occur parallel to the grain boundary – eventually grain boundary will simply fall out!!
20Design for Intergranular Attack: Watch welding of stainless steels (causes sensitization). Always anneal at 1900 – 2000 F after welding to redistribute Cr.Use low carbon grade stainless to eliminate sensitization (304L or 316L).Add alloy stabilizers like titanium which ties up the carbon atoms and prevents chromium depletion.Mostly in the material chemistry.
22Example 2: Intergranular Attack: Exfoliation of high strength Aluminum alloys.Corrosion that preferentially attacts the elongated grains of rolled aluminum.Corroded grains usually near surfaceGrain swells due to increase in volume which causes drastic separation to occur in a pealing fashion.
23Dealloying:When one element in an alloy is anodic to the other element.Example: Removal of zinc from brass (called dezincification) leaves spongy, weak brass.Brass alloy of zinc and copper and zinc is anodic to copper (see galvanic series).
24Dealloying: Danger! The alloy may not appear damaged May be no dimensional variationsMaterial generally becomes weak – hidden to inspection!
25Dealloying: Two common types: Dezincification – preferential removal of zinc in brassTry to limit Zinc to 15% or less and add 1% tin.Cathodic protectionGraphitization – preferential removal of Fe in Cast Iron leaving graphite (C).
26Erosion: Basically a repeat of Chapter 3 (see- Erosion Wear) Forms of Erosion:Liquid ImpingementLiquid erosionSlurry ErosionCavitationRead definitions on page 523.
27Methods to Control Corrosion There are five methods to control corrosion:material selectioncoatingschanging the environmentchanging the potentialdesignretyped
28How to avoid (or control) Corrosion? Material Selection! Remember – environment key. Look at potential pH diagrams!!!Eliminate any one of the 4 req’ments for corrosion!Galvanic - Avoid using dissimilar metals.Or close together as possibleOr electrically isolate one from the otherOr MAKE ANODE BIG!!!
29How to avoid (or control) Corrosion? Pitting/Crevice: Watch for stagnate water/ electrolyte.Use gasketsUse good welding practicesIntergranular – watch grain size, environment, temperature, etc.. Careful with Stainless Steels and AL.
30How to avoid (or control) Corrosion? Consider organic coating (paint, ceramic, chrome, etc.) – DANGER IF IT GETS SCRACTHED!!OR BETTER YET, consider cathodic protection:such as zinc (or galvanized) plating on steelMg sacrificial anode on steel boat hullImpressed current, etc..
31Corrosion Control:Anodic Protection – Zinc coating of steel. KNOW HOW THIS WORKS!!
33DESIGN for CorrosionBracket easier to replace than pipe!
34Surface Treatment (Coatings) Organic paintsChromating and phosphating:The Process - chromating and phosphating are surface-coating processes that enhance the corrosion resistance of metals. Both involve soaking the component in a heated bath based on chromic or phosphoric acids. The acid reacts with the surface, dissolving some of the surface metal and depositing a thin protective layer of complex chromium or phosphorous compoundsAnodizing (aluminum, titanium)The Process - Aluminum is a reactive metal, yet in everyday objects it does not corrode or discolor. That is because of a thin oxide film - Al2O3 - that forms spontaneously on its surface, and this film, though invisible, is highly protective. The film can be thickened and its structure controlled by the process of anodizing. The process is electrolytic; the electrolyte, typically, is dilute (15%) sulfuric acid. Anodizing is most generally applied to aluminum, but magnesium, titanium, zirconium and zinc can all be treated in this way. The oxide formed by anodizing is hard, abrasion resistant and resists corrosion well. The film-surface is micro-porous, allowing it to absorb dyes, giving metallic reflectivity with an attractive gold, viridian, azure or rose-colored sheen; and it can be patterned. The process is cheap, an imparts both corrosion and wear resistance to the surface.See – corrosion and surface treatment word document
35Surface Treatment (Coatings) Electro-platingThe Process -Metal coating process wherein a thin metallic coat is deposited on the workpiece by means of an ionized electrolytic solution. The workpiece (cathode) and the metallizing source material (anode) are submerged in the solution where a direct electrical current causes the metallic ions to migrate from the source material to the workpiece. The workpiece and source metal are suspended in the ionized electrolytic solution by insulated rods. Thorough surface cleaning precedes the plating operation. Plating is carried out for many reasons: corrosion resistance, improved appearance, wear resistance, higher electrical conductivity, better electrical contact, greater surface smoothness and better light reflectance.BluingBluing is a passivation process in which steel is partially protected against rust, and is named after the blue-black appearance of the resulting protective finish. True gun bluing is an electrochemical conversion coating resulting from an oxidizing chemical reaction with iron on the surface selectively forming magnetite (Fe3O4), the black oxide of iron, which occupies the same volume as normal iron. Done for bolts called “blackening”Hot-dip Coating (i.e. galvanizing)Hot dipping is a process for coating a metal, mainly ferrous metals, with low melting point metals usually zinc and its alloys. The component is first degreased in a caustic bath, then pickled (to remove rust and scale) in a sulfuric acid bath, immersed (dipped) in the liquid metal and, after lifting out, it is cooled in a cold air stream. The molten metal alloys with the surface of the component, forming a continuous thin coating. When the coating is zinc and the component is steel, the process is known as galvanizing.The process is very versatile and can be applied to components of any shape, and sizes up to 30 m x 2 m x 4 m. The cost is comparable with that of painting, but the protection offered by galvanizing is much greater, because if the coating is scratched it is the zinc not the underlying steel that corrodes ("galvanic protection"). Properly galvanized steel will survive outdoors for years without further treatment.Discuss and show Bolts!!!
36Which one is galvanized and which one is chrome plated?
37Material Selection: Importance of Oxide films The fundamental resistance of stainless steel to corrosion occurs because of its ability to form an oxide protective coating on its surface. This thin coating is invisible, but generally protects the steel in oxidizing environments (air and nitric acid). However, this film loses its protectiveness in environments such as hydrochloric acid and chlorides. In stainless steels, lack of oxygen also ruins the corrosion protective oxide film, therefore these debris ridden or stagnant regions are susceptible to corrosion.
38The “Right” material depends on the environment. Polarization can have a major effect on metal stability.Recall CES Rankings: strong acid, weak acid, water, weak alkali, strong alkali
40Often several approaches to control corrosion Often several “system” constraints pertain
41Cathodic Protection (CP) Cathodic protection (CP) is a technique to control the corrosion of a metal surface by making it work as a cathode of an electrochemical cell. This is achieved by placing in contact with the metal to be protected another more easily corroded metal to act as the anode of the electrochemical cell. Cathodic protection systems are most commonly used to protect steel, water or fuel pipelines and storage tanks, steel pier piles, ships, offshore oil platforms and onshore oil well casings.Types of CP:sacrificial anodes – zinc, magnesium or aluminum. The sacrificial anodes are more active (more negative potential) than the metal of the structure they’re designed to protect. The anode pushes the potential of the steel structure more negative and therefore the driving force for corrosion halts. The anode continues to corrode until it requires replacement,Impressed current CP – done for large structures (pipes, offshore platforms, etc) where a galvanic (or sacrificial) anode can not economically deliver enough current.Galvanized steel (see above slide) – again, steel is coated with zinc and if the zinc coating is scratched and steel exposed, the surrounding areas of zinc coating form a galvanic cell with the exposed steel and protects in from corroding. The zinc coating acts as a sacrificial anode.Bob, discuss difference between cathodic and anodic protection